Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts
no text concepts found
Transcript
```Resistivity and Carrier Transport Parameters in Silicon
Virginia Semiconductor, Inc.
1501 Powhatan Street, Fredericksburg, VA 22401
(540) 373-2900, FAX (540) 371-0371
www.vriginiasemi.com, [email protected]
A Introduction
This paper contains information on the resistivity, mobility, and diffusivity of electrons
and holes in silicon. It also contains information on minority carrier lifetimes and
diffusion lengths.
In general, carrier lifetimes and diffusion lengths must be measured experimentally, but
the equations and values given in the paper are reasonable approximations for resistivities
B Resistivity, Mobility, and Diffusivity for n-type and p-type doped silicon
In one dimension, the current density of electrons can be approximated with the
following equation

 dn
Jn = ( n ⋅ q ⋅ u n ⋅ E ) +  q ⋅ D n 
 dx


 

(Amps/cm2)
(1) [1]
where “q” is the charge, “un” is the mobility, “E” is the electric field, “Dn” is the diffusion
coefficient, n is the carrier concentration (c), and
n ≈ ND = c
at 300K (ohm-cm).
The current density of holes is given by a similar equation

 dp
Jp = (p ⋅ q ⋅ u p ⋅ E ) −  q ⋅ D p 
 dx


 

(Amps/cm2)
(2) [1]
where
p ≈ NA = c
at 300K (ohm-cm).
The resistivity is,
p=
1
1
1
.
=
=
c ⋅q ⋅u NA ⋅q ⋅up
N D ⋅ q ⋅ un
For J ≈ 0, and equilibrium conditions
Dn
k ⋅T
=
u
q
(4)
(3)
where k is the Boltzmann constant.
Tables 1,2 use the above equations 3,4 for u and D, as well as the data from reference [2].
High resistivity silicon can only be produced using the Float Zone (FZ) crystal growth
method. The FZ method does not use a crucible during crystal growth. The Czochralski
(CZ) method uses a quartz crucible during crystal growth, and oxygen from the crucible
dopes the material. The unintentional oxygen dopant behaves as an n-type impurity and
precludes solidification of oxygen-free material and high resistivity. Intentional dopants
are introduced to FZ material during solidification using doping gases. This limits the
maximum concentration of doping during the FZ method. The typical p-type impurity
for silicon is Boron. Although, Gallium doping has been used for certain applications
related to solar cells. Silicon is doped n-type using Phosphorous, Arsenic, or Antimony.
Low resistivity n-type material is achieved using Arsenic doping.
P
(ohm-cm)
0.0001
0.001
0.01
0.1
1
10
100
1000
10000
n (cm-3)
1.60E+21
7.38E+19
4.53E+18
7.84E+16
4.86E+15
4.45E+14
4.27E+13
4.20E+12
4.00E+11
ND (cm-3)
1.60E+21
7.38E+19
4.53E+18
7.84E+16
4.86E+15
4.45E+14
4.27E+13
4.20E+12
4.00E+11
un
(cm2/(V-s))
Dn
(cm2/s)
39.063
84.688
137.969
797.194
1286.008
1404.494
1463.700
1488.095
1562.500
1.011
2.191
3.570
20.627
33.275
36.341
37.873
38.504
40.430
Grow Method
Cz
Cz
Cz
Cz
Cz,Fz
Cz,Fz
Cz,Fz
Fz
Fz
Table 1 shows electron properties in n-type Si at 300K [2]
P
(ohm-cm)
0.0001
0.001
0.01
0.1
1
10
100
1000
10000
p (cm-3)
1.20E+21
1.70E+20
8.49E+18
2.77E+17
1.46E+16
1.34E+15
1.33E+14
1.30E+13
1.30E+12
NA (cm-3)
1.20E+21
1.70E+20
8.49E+18
2.77E+17
1.46E+16
1.34E+15
1.33E+14
1.30E+13
1.30E+12
up
(cm2/(V-s))
Dp
(cm2/s)
52.083
36.765
73.616
225.632
428.082
466.418
469.925
480.769
480.769
1.348
0.951
1.905
5.838
11.077
12.069
12.159
12.440
12.440
Grow Method
Cz
Cz
Cz
Cz
Cz,Fz
Cz,Fz
Cz,Fz
Fz
Fz
Table 2 shows hole properties in p-type Si at 300K [2]
C Electron and Hole Minority Carrier Lifetime and Diffusion Lengths
The electron minority carrier diffusion length in p-type Si is approximated by
Le=
 kT 
 u eτ e
 q 
cm
(5)[1][2][3]
where k is the Boltzmann constant, T is the absolute temperature (K), q is the charge, ue
is the electron mobility, and τ e is the electron minority carrier lifetime estimated by
1
τe
[(
)]
) (
= 3.45 × 10 −12 N a + 9.5 × 10 −32 N a2 s −1
(6)[1][2][3]
where Na is the acceptor density and Na > 1 x 1017 (cm-3). The hole diffusion length in ntype Si is given by
Lh=
 kT 
 u hτ h
 q 
cm
(7)[1][2][3]
where k is the Boltzmann constant, T is the absolute temperature (K), q is the charge, uh
is the hole mobility, and τ h is the hole lifetime estimated by
1
τh
[(
) (
)]
= 7.8 × 10 −13 N d + 1.8 × 10 −31 N d2 s −1
(8)[2][3]
where Nd is the donator density and Nd > 1 x 1017 (cm-3).
Tables 3,4 use the above equations to estimate the minority carrier properties in silicon at
300K.
ND (cm-3)
1.60E+21
7.38E+19
4.53E+18
7.84E+16
Th s-1
2.164E-12
9.635E-10
1.384E-07
1.606E-05
Lh cm
1.708E-06
3.029E-05
5.136E-04
9.687E-03
Table 3 shows Lifetimes and Diffusion Lengths of hole Minority Carriers [2]
NA (cm-3)
1.20E+21
1.70E+20
8.49E+18
2.77E+17
Te s-1
7.095E-12
3.001E-10
2.767E-08
1.038E-06
Le cm
2.679E-06
2.565E-05
3.144E-04
4.630E-03
Table 4 shows Lifetimes and Diffusion Lengths of electron Minority Carriers [2]
Lifetimes for high resistivity material are difficult to predict and widely varying
depending on the FZ or CZ technique used. Direct experimental measurement is
generally required to estimate the carrier lifetime in high resistivity material. The
lifetime is controlled by the total concentration Na+Nd, while the resistivity is controlled
by the difference in dopants, Na-Nd. At high resistivities Na-Nd is very small, but
Na+Nd can be large and widely varying for a given resistivity. The opposite is true at
low resistivity making estimation of the lifetime more consistent.
D Summary
This paper contains estimations of silicon resistivity, as well as carrier mobility, and
diffusivity for electrons and holes at 300K. It also contains information on minority
carrier lifetimes and diffusion lengths. The reader is directed to reference [2] for further
details related to temperature, electric field, and processing dependencies to the resistivity
and transport properties.
E References
[1]
[2]
[3]
S.M. Sze [ Physics of Semiconductor Devices (John Wiley and Son s, Inc,
New York, 1981)]
R. Hull [ Properties of Crystalline Silicon (INSPEC, London, 1999)]
D. Huber, A. Bachmeier, R. Wahlich, H. Herzer [Proc. Conf. Semiconductor
Silicon 1986 Eds. H.R. Huff, T. Abe, B. Kobessen (Electrochemical Society,
USA, 1986) p.1022-32]
```
Related documents